Electromechanical Behavior of Chemically Reduced Graphene Oxide and Multi-walled Carbon Nanotube Hybrid Material
© Benchirouf et al. 2016
Received: 27 October 2015
Accepted: 22 December 2015
Published: 5 January 2016
In this paper, we propose strain-sensitive thin films based on chemically reduced graphene oxide (GO) and multi-walled carbon nanotubes (MWCNTs) without adding any further surfactants. In spite of the insulating properties of the thin-film-based GO due to the presence functional groups such as hydroxyl, epoxy, and carbonyl groups in its atomic structure, a significant enhancement of the film conductivity was reached by chemical reduction with hydro-iodic acid. By optimizing the MWCNT content, a significant improvement of electrical and mechanical thin film sensitivity is realized. The optical properties and the morphology of the prepared thin films were studied using ultraviolet-visible spectroscopy (UV-Vis) and scanning electron microscope (SEM). The UV-Vis spectra showed the ability to tune the band gap of the GO by changing the MWCNT content, whereas the SEM indicated that the MWCNTs were well dissolved and coated by the GO. Investigations of the piezoresistive properties of the hybrid nanocomposite material under mechanical load show a linear trend between the electrical resistance and the applied strain. A relatively high gauge factor of 8.5 is reached compared to the commercial metallic strain gauges. The self-assembled hybrid films exhibit outstanding properties in electric conductivity, mechanical strength, and strain sensitivity, which provide a high potential for use in strain-sensing applications.
KeywordsMulti-walled carbon nanotubes Graphene oxide Chemical reduction Piezoresistivity Strain sensor
In the last decade, the increasing trend towards flexible electronic devices emphasizes their attractive perspective in numerous applications. Essential components in such multifunctional devices are sensors, which should be flexible, scalable, sensitive, and robust for integration. Due to their promising electrical and mechanical properties, carbon nanotubes (CNTs) are promising nanomaterials for realization of strain sensors with high performance. Carbon-nanomaterial-filled composites have been intensively studied as multifunctional material for numerous smart applications. Strain sensors among others have especially attracted a lot of interest [1–11]. Basically, the induced strain alters the electrical resistance of a randomly distributed CNT network. The change of the electrical resistance results from the modification of contact arrangements and the tunneling distance between the CNTs [10, 12–15]. Many scientists reported the use of CNT-filled polymer nanocomposites for strain-sensing [7–9, 11–15]. Among others, polydimethylsiloxane (PDMS) [16–18], polyvinyl alcohol (PVA) [8, 19], and epoxy [8, 20, 21] are considered as promising nanocomposites due to the possibility to modify its strain range by controlling the filler content and filler orientation. However, some difficulties on tailoring the strain sensitivity and mechanical properties of the strain-sensor-based thin films such as the influence of processing parameters and orientation of the CNTs within the polymer matrix were broadly reported [10, 14]. Recently, colloid dispersions and thin-film-based graphene, graphene oxide (GO), and reduced graphene oxide (rGO) films have been widely produced and characterized [22–33]. The investigations pointed out to use them as electrocatalytic materials , supercapacitors , and transparent electrodes [24, 28, 31]. Nevertheless, their electromechanical properties have not yet been well addressed. GO can be principally used as a dispersant to suspend the agglomerated CNTs in water and to develop a new solution-processing strategy for making GO:CNT hybrid nanocomposites. Compared with pristine multi-walled carbon nanotubes (MWCNTs), such a nanocomposite can be well dispersed in an aqueous solution via the π-π interaction, which stabilizes not only the hydrophobic nanotubes but also provides the MWCNTs with a negative charge [26, 27, 30, 36–38]. Therefore, CNTs dispersed in GO dispersion are expected to have interesting mechanical properties, due to the exceptional mechanical properties of both GO and CNTs.
Properties of the pristine GO and its composites have been widely studied. Wang et al. prepared transparent conductive films based on rGO:SWCNT using a filtration method. The electrical conductivity was improved by a factor of 4–13 after chemical reduction. Besides the electrical properties, X-ray photoelectron spectroscopy (XPS) was used to determine the content of carbon, oxygen, and other elements in the film before and after the chemical reduction . Suk et al. investigated the mechanical properties of the mono-, double, and triple layer of GO using an atomic force microscopy (AFM). The monolayer of the GO had an effective Young’s modulus of 207.6 ± 23.4 GPa . Liu et al. fabricated rGO:CNT using a catalyst-free route method and studied systematically its thermostability, photoluminescence, and electrical properties. The obtained results revealed that introducing CNT to GO improved all the prementioned properties and therefore suggest a high potential application in the field of photonics and electrical devices . Wang et al. reported a synergetic improvement in the electrical and mechanical strength when composite fibers of graphene oxide:single-walled carbon nanotubes (GO:SWCNT) were fabricated by PVA-based coagulation spinning technique . Liu et al. used the first-principle computations to simulate and predict the mechanical properties of the monolayer of GO. He proved that the ordered GO has a Young’s modulus between 380 and 470 GPa, which is higher than the amorphous GO. The change in the Young’s modulus is mainly related to the oxygen coverage, whereas higher coverage leads to lower the Young’s modulus and vice versa . Kotal and Bhowmick made a very detailed investigation of MWCNT chemically bonded to rGO using a wide variety of methods: infrared, Raman, ultraviolet-visible (UV-Vis), X-ray diffraction, XPS, scanning electron microscope (SEM), transmission electron microscopy (TEM), and scanning tunneling microscopy (STM). They found out that the proposed hybrid material exhibits excellent electrical and thermal properties, which made it an excellent candidate for potential energy storage applications such as supercapacitors . Hwang et al. fabricated a transparent thin-film-based rGO with tuned piezoresistivity. The films were reduced using two different methods: (i) temperature and (ii) hydrazine. The manufactured rGO films reduced using hydrazine showed a higher gauge factor (around 8.67) than films reduced using temperature . Trung et al. introduced a new type of flexible strain sensor array based on the rGO field effect transistor (FET), which is able to determine a very small tensile and compression strain of 0.02 %, excellent repeatability up to 10,000 bending cycles, and with fast response and relaxation time . Hwang et al. improved the thermal and mechanical properties of the GO by the addition of the MWCNTs. They stated that amino-functionalized MWCNT bonded to GO exhibits synergetic thermal and mechanical properties compared to the non-functionalized MWCNT .
The aim of the present work is to show the feasibility of fabricating the rGO:MWCNT nanocomposite films on a flexible substrate for strain-sensing applications. In this paper, a hybrid nanomaterial GO:MWCNT is synthesized based on the self-assembly of GO and MWCNTs. The nanocomposite films should be highly sensitive to strain, and therefore, its performance should be improved by optimizing the material composition. This can be realized based on the understanding of optical and morphological, as well as the electromechanical, properties of the nanocomposites.
where σ is the thin film conductivity and R is the ohmic resistance; A and L are cross-section area and the thin film length, respectively.
For strain measurements, the samples were stretched using a tensile-compressive cyclic (TCC) machine (Inspekt 10 table from Hegewald & Peschke, Meß- und Prüftechnik GmbH). The setup for the strain measurement is shown elsewhere . The range of the applied force was varied from 0 to 110 N with a step size of 10 N for loading and unloading at a speed of 1 mm/min. At each step force, the I-V characteristics were measured by applying voltage from −0.5 to 0.5 V and the resulting current was recorded by a Keithley 2602 SourceMeter (Keithley Instruments Inc., Cleveland, OH, USA) connected to a host computer through GPIB/USB cable and coupled with the TCC.
Results and Discussion
where A is the absorbance, α is the absorption coefficient, t is the cuvette thickness, and C is the concentration.
A linear relationship between the absorbance and the MWCNT concentration (C) was extracted, while the absorption coefficient (α) was calculated to be approximately 800 L/(g m).
where ΔR and R 0 are the change of the sensor’s resistance and initial resistance (at ε = 0), respectively.
The sensitivity of the thin films decreased with increasing MWCNT content, which is in agreement with the previous works [10, 14]. The average strain sensitivity was 8.5 for 0.01 wt.% and 1.23 for 0.05 wt.% MWCNTs (Supplementary data). The piezoresistivity of the rGO:MWCNT thin films under strain could be explained as a superposition of the following aspects: (i) For rGO, the increase of the resistance is mainly due to the elongation of the bond length between the C atoms in the benzene ring under strain [39, 42]; (ii) For the MWCNTs, the reorientation and the change in the tunneling distance between the adjacent CNTs; and (iii) The change in the number of tunneling contacts formed between the rGO and MWCNT within the conduction network significantly change the total thin film resistance under strain.
In this paper, we demonstrated the feasibility of realization of rGO:MWCNT nanocomposite films on a flexible substrate for potential use in strain sensor applications. The optical, morphological, and electromechanical properties were investigated for the thin films with different amount of MWCNTs. The UV-Vis spectra show an increase in the absorption as the MWCNT content increases and the tunability of the GO band gap as a function of the MWCNT loading. Electron microscopy results show that the MWCNTs are well dispersed in the GO, forming a uniform dense network. The dependency of the MWCNT amount on both the electrical resistivity and the mechanical properties was investigated. Lower MWCNT content in the GO matrix shows higher sensitivity due to the higher tunneling effect between the neighboring tubes and the shrinkage of the rGO band gap. The reached results are promising for the realization of strain sensors with a high sensitivity reaching a gauge factor of 8.5. We claim that further optimization and improvement of the hybrid composite could be possible to achieve better electrical and mechanical properties in the field of strain-sensing application.
A. Benchirouf would like to thank Dr. Cristina Valles from the University of Manchester for the fruitful discussion and support, Ravikant Sharma for the tips to improve the graphics, and Torsten Jagemann and Prof. Michael Hietschold from Chair of Solid Surfaces Analysis at Technische Universität Chemnitz for permitting us to use the SEM.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Tombler T, Zhou X, Alexseyev L, Kong J, Dai H, Liu L, Jayanthi C, Tang M, Wu S (2000) Reversible electromechanical characteristics of carbon nanotubes under local-probe manipulation. Nature 405:769–772View ArticleGoogle Scholar
- Dharap P, Li Z, Nagarajaiah S, Barrera E (2004) Nanotube film based on single-wall carbon nanotubes for strain sensing. Nanotechnology 15:379–382View ArticleGoogle Scholar
- Grow R, Wang Q, Cao J, Wang D, Dai H (2005) Piezo-resistance of carbon nanotubes on deformable thin-film membranes. Applied Physic s Letters 86(9):3, Article ID 093104Google Scholar
- Kang I, Schulz M, Kim J, Shanov V, Shi D (2006) A carbon nanotube strain sensor for structural health monitoring. Smart Mater Struct 15:737–748View ArticleGoogle Scholar
- Li X, Levy C, Elaadil L (2008) Multiwalled carbon nanotube film for strain sensing. Nanotechnology 19(4): 045501-045508Google Scholar
- Chang F, Wang R, Yang H, Lin Y, Chen T, Huang S (2010) Flexible strain sensors fabricated with carbon nano-tube and carbon nano-fiber composite thin films. Thin Solid Films 518:7343–7347View ArticleGoogle Scholar
- Yin G, Hu N, Karube Y, Liu Y, Li Y, Fukunaga H (2011) A carbon nanotube/polymer strain sensor with linear and anti-symmetric piezoresistivity. J Compos Mater 45:1315–1323View ArticleGoogle Scholar
- Alamusi Y, Surina L, Hu N, Ning H, Liu Y, Wu L, Atobe S, Fukunaga H (2013) Ultrasensitive strain sensors of multiwalled carbon nanotube/epoxy nanocomposite using dielectric loss tangent. Appl Phys Lett 103(22):221903View ArticleGoogle Scholar
- Benchirouf A, Sanli A, El-Houdaigui I, Bashorun M, Ciers J, Müller C, Kanoun O (2014) Evaluation of the piezoresistive behavior of multifunctional nanocomposites thin films, 11th international multi-conference on systems, signals & devices., pp 11–14Google Scholar
- Kanoun O, Müller C, Benchirouf A, Sanli A, Dinh TN, Al-Hamry A, Bu L, Gerlach C, Bouhamed A (2014) Flexible carbon nanotube films for high performance strain sensors. Sensors 14(6):10042–10071View ArticleGoogle Scholar
- Amjadi M, Yoon Y, Park I (2015) Ultra-stretchable and skin-mountable strain sensors using carbon nanotubes–Ecoflex nanocomposites. Nanotechnology 26(37):375501View ArticleGoogle Scholar
- Wang P, Geng S, Ding T (2010) Effects of carboxyl radical on electrical resistance of multi-walled carbon nanotube filled silicone rubber composite under pressure. Compos Sci Technol 70(10):1571–1573View ArticleGoogle Scholar
- Yasuoka T, Shimamura Y, Todoroki A (2010) Electrical resistance change under strain of CNF/flexible-epoxy composite. Adv Compos Mater 19:123–138View ArticleGoogle Scholar
- Obitayo W, Liu T (2012) A review: carbon nanotube-based piezoresistive strain sensors. J Sensors 2012:15, Article ID 652438View ArticleGoogle Scholar
- Hu N, Karube Y, Arai YM, Watanabe T, Yan C, Li Y, Liu Y, Fukunaga H (2010) Investigation on sensitivity of a polymer/carbon nanotube composite strain sensor. Carbon 48:680–687View ArticleGoogle Scholar
- Lipomi D, Vosgueritchian M, Tee B, Hellstrom S, Lee J, Fox C, Bao Z (2011) Skin-like pressure and strain sensors based on transparent elastic films of carbon nanotubes. Nat Nanotechnol 6:788–792View ArticleGoogle Scholar
- Lu N, Lu C, Yang S, Rogers J (2012) Highly sensitive skin-mountable strain gauges based entirely on elastomers. Adv Funct Mater 22(19):4044–4050View ArticleGoogle Scholar
- Amjadi M, Park I (2014) Sensitive and stable strain sensors based on the wavy structured electrodes. Proceedings of the 14th IEEE International conference on nanotechnology, Toronto, Canada, August 18–21View ArticleGoogle Scholar
- Kumar S, Singh D, Nisha M (2015) Resistance based damage sensing in electrically non conductive composites using carbon nanotubes. Int J Innov Sci Eng Technol 2(1): 640-651 Google Scholar
- Wichmann M, Buschhorn S, Böger L, Adelung R, Schulte K (2008) Direction sensitive bending sensors based on multi-wall carbon nanotube/epoxy nanocomposites. Nanotechnology 19(48):475503-475507 Google Scholar
- Rams T, Sanchez M, Urena A, Jimenez-Suarez A, Campo M, Guemes A (2012) Use of carbon nanotubes for strain and damage sensing of epoxy-based composites. Int J Smart Nano Materials 3(2):152-161 Google Scholar
- King P, Khan U, Lotya M, De S, Coleman N (2010) Improvement of transparent conducting nanotube films by addition of small quantities of graphene. ACS Nano 4:4238–46View ArticleGoogle Scholar
- Hong T, Lee D, Choi H, Shin H, Kim B (2010) Transparent, flexible conducting hybrid multilayer thin films of multiwalled carbon nanotubes with graphene nanosheets. ACS Nano 4:3861–3868View ArticleGoogle Scholar
- Guo X, Liu X, Lin F, Li H, Fan Y, Zhang N (2015) Highly conductive transparent organic electrodes with multilayer structures for rigid and flexible optoelectronics. Scientific reports (5):10569 Google Scholar
- Zhang Q, Yang S, Zhang J, Zhang L, Kang P, Li J (2011) Fabrication of an electrochemical platform based on the self-assembly of graphene oxide-multiwall carbon nanotube nanocomposite and horseradish peroxidase: direct electrochemistry and electrocatalysis. Nanotechnology 22:494010View ArticleGoogle Scholar
- Chua C, Pumera M (2014) Chemical reduction of graphene oxide: a synthetic chemistry viewpoint. Chem Soc Rev 43(1): 13774-13779 Google Scholar
- Konios D, Stylianakis M, Stratakis E, Kymakis E (2014) Dispersion behaviour of graphene and reduced graphene oxide. J Colloid Interface Sci 430:108–112View ArticleGoogle Scholar
- Zhenga Q, Li Z, Yang J, Kim J (2014) Graphene oxide-based transparent conductive films. Prog Mater Sci 64:200–247View ArticleGoogle Scholar
- Wang R, Sun J, Gao L, Xu C, Zhang J, Liu Y (2011) Effective post treatment for preparing highly conductive carbon nanotube/reduced graphite oxide hybrid films. Nanoscale 3:904–6View ArticleGoogle Scholar
- Tian L, Meziani M, Lu F, Kong C, Cao L, Thorne T (2010) Graphene oxides for homogeneous dispersion of carbon nanotubes. ACS Appl Mater Interf 2:3217–22View ArticleGoogle Scholar
- Hwang S, Ahn H, Yoon J, Jang J, Park Y (2013) Transparent graphene films with a tunable piezoresistive response. J Mater Chem C 1(43)Google Scholar
- Hidalgo R, López-Díaz D, Velázquez M (2015) Graphene oxide thin films: influence of chemical structure and deposition methodology. Langmuir 31(9):2697–2705View ArticleGoogle Scholar
- Cano M, Khan U, Sainsbury T, O’Neill A, Wang Z, McGovern I, Maser W, Benito A, Coleman J (2013) Improving the mechanical properties of graphene oxide based materials by covalent attachment of polymer chains. Carbon 52:363–371View ArticleGoogle Scholar
- Han P, Yue Y, Liu Z, Xu W, Zhang L, Xu H (2011) Graphene oxide nanosheets/multi-walled carbon nanotubes hybrid as an excellent electrocatalytic material towards VO2+/VOfl2 redox couples for vanadium redox flow batteries. Energy Environ Sci 4:4710–7View ArticleGoogle Scholar
- Huang Z, Zhang B, Zheng O, Lin X, Yousefi N (2012) Self-assembled reduced graphene oxide carbon nanotube thin films as electrode for supercapacitors. J Mater Chem 22:3591–9View ArticleGoogle Scholar
- Qiu L, Yang X, Gou X, Yang W, Ma Z, Wallace G, Li D (2010) Dispersing carbon nanotubes with graphene oxide in water and synergistic effects between graphene derivatives. Chem Eur J 16:10653–10658View ArticleGoogle Scholar
- Cai D, Song M, Xu C (2008) Highly conductive carbon-nanotube/graphite-oxide hybrid films. Adv Mater 20(9):1706–9View ArticleGoogle Scholar
- Zhang C, Ren L, Wang X, Liu T (2010) Graphene oxide-assisted dispersion of pristine multiwalled carbon nanotubes in aqueous media. J Phys Chem C 114:11435–11440View ArticleGoogle Scholar
- Suk J, Piner R, An J, Ruoff R (2010) Mechanical properties of monolayer graphene oxide. ACS Nano 4(11):6557–6564View ArticleGoogle Scholar
- Liu F, Cao Y, Yi M, Xi L, Huang W, Tang N, Zhong W, Du Y (2013) Thermostability, photoluminescence, and electrical properties of reduced graphene oxide–carbon nanotube hybrid materials. Crystals 3:28–37View ArticleGoogle Scholar
- Wang R, Dun J, Gao L, Xu C, Zhang J (2011) Fibrous nanocomposites of carbon nanotubes and graphene-oxide with synergetic and actuative performance. Chem Comm 47:8650–8652View ArticleGoogle Scholar
- Liu L, Zhang J, Zhao J, Liu F (2012) Mechanical properties of graphene oxides. Nanoscale 4(19):5910–6View ArticleGoogle Scholar
- Kotal M, Bhowmick A (2013) Multifunctional hybrid materials based on carbon nanotube chemically bonded to reduced graphene oxide. J Phys Chem C 117:25865–25875View ArticleGoogle Scholar
- Trung T, Tien N, Kim D, Jang M, Yoon O, Lee N (2013) A flexible reduced graphene oxide field-effect transistor for ultrasensitive strain sensing. Adv Funct Mater 24(1):117–124 Google Scholar
- Hwang Y, Kim M, Kim J (2013) Enhancement of thermal and mechanical properties of flexible graphene oxide/carbon nanotube hybrid films though direct covalent bonding. J matter sci 48:7011–7021View ArticleGoogle Scholar
- Hintze P, Kjaergaard H, Vaida V, Burkholder J (2003) Vibrational and electronic spectroscopy of sulfuric acid vapor. J Phys Chem A 107:1112–1118View ArticleGoogle Scholar
- Loh K, Bao Q, Eda G, Chhowalla M (2010) Graphene oxide as a chemically tunable platform for optical applications. Nat Chem 2(12):1015–24View ArticleGoogle Scholar
- Pei S, Zhao J, Du J, Ren W, Cheng H (2010) Direct reduction of graphene oxide films into highly conductive and flexible graphene films by hydrohalic acids. Carbon 48(15):4466–4474View ArticleGoogle Scholar